NOTCHES AND THEIR EFFECTS. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1


 Anne May
 3 years ago
 Views:
Transcription
1 NOTCHES AND THEIR EFFECTS Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1
2 CHAPTER OUTLINE Background Stress/Strain Concentrations SN Approach for Notched Members StrainLife Approach for Notched Members Applications of LEFM to FCG at Notches The TwoStage Approach Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 2
3 BACKGROUND Notches cannot be avoided in many structures and machines and notch effects have been a key problem in the study of fatigue. Examples: Thread roots and the transition between the head and the shank Rivet holes in sheets Welds on plates Keyways on shafts Although notches can be very dangerous they can often be rendered harmless by suitable treatment. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 3
4 BACKGROUND To understand the effects of notches one must consider five parameters: 1. Concentrations of stress and of strain. 2. Stress gradients. 3. Mean stress effects and residual stresses. 4. Local yielding. 5. Development and growth of cracks. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 4
5 STRESS AND STRAIN CONCENTRATIONS AND GRADIENTS The degree of stress and strain concentration is a factor in the fatigue strength of notched parts. It is measured by the elastic stress concentration factor, K t : K t S e As long as / = constant = E Where: or = the maximum stress or strain at the notch S or e = the nominal stress or strain Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 5
6 STRESS AND STRAIN CONCENTRATIONS AND GRADIENTS K t plotted vs the ratio of hole diameter to sheet width. In the upper curve the nominal stress is defined as load divided by total or gross area (w x t). In the lower curve the nominal stress is defined as load divided by net area. In this book we use the net area to define the nominal stress when using stress concentration factors. However, in calculating the stress intensity factor from the nominal stress we use the gross area as if the crack did not exist, as in Ch 6. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 6
7 STRESS AND STRAIN CONCENTRATIONS AND GRADIENTS Figure 7.2 shows stresses near a circular hole in the center of a wide sheet in tension. The following equations represent the axial stress y and the transverse stress x : S S y x r x r x 2 S = nominal stress = load/area y = axial stress x = transverse stress x = distance from center of hole r = radius of hole r x r x 4 4 Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 7
8 STRESS AND STRAIN CONCENTRATIONS AND GRADIENTS Values of y /S and x /S are plotted versus x/r. y /S decreases quite rapidly as the distance from the edge of the hole is increased. K t at the edge of the hole is 3, while at a distance of 0.25r the value of y /S is only about 2. At a distance of 2r it is only Rapid decrease of stress with increasing distance from the notch and existence of biaxial or triaxial states of stress at a small distance from the notch are typical of stress concentrations. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 8
9 STRESS AND STRAIN CONCENTRATIONS AND GRADIENTS For deep narrow notches with semicircular ends a formula analogous to linear elastic fracture mechanics formulas has been given for the stress distribution: r y max 0.5r 0.5r d 1 / 2 d where d is the distance from the edge of the notch of radius r. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 9
10 STRESS AND STRAIN CONCENTRATIONS AND GRADIENTS The stress concentration produced by a given notch is not a unique number as it depends on the mode of loading. For instance, for the circular hole in a wide sheet: In tension: 3 In biaxial tension: 2 Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 10
11 STRESS AND STRAIN CONCENTRATIONS AND GRADIENTS Elastic stress concentration factors are obtained from: Theory of elasticity Numerical solutions Experimental measurements The most common and flexible numerical method is the finite element method. A model with relatively fine mesh in the areas of steep stress gradients is required. Experimental measurement techniques widely used include Brittle coatings Photoelasticity Thermoelasticity Strain gages. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 11
12 STRESS AND STRAIN CONCENTRATIONS AND GRADIENTS Brittle Coating Technique: A brittle coating is sprayed on the surface and allowed to dry. Crack patterns developed by the loading and their relation to a calibration coating indicate regions and magnitudes of stress concentrations. Photoelasticity Technique: A specimen with identical geometry to the actual notched part is made of a certain transparent material. Changes in optical properties of the transparent material under load, measured by a polariscope, indicate stress distributions and magnitudes. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 12
13 STRESS AND STRAIN CONCENTRATIONS AND GRADIENTS Thermoelasticity Technique: Stress distribution is obtained by monitoring small temperature changes of the specimen or component subjected to cyclic loading. Electrical Resistance Strain Gage: The most common experimental measurement technique A strain gage is bonded to the surface in the region of interest. Applied load causes dimensional changes of the gage resulting in changes to electrical resistance, which in turn indicates the existing strain. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 13
14 STRESS AND STRAIN CONCENTRATIONS AND GRADIENTS Charts of stress concentration factors are available in the literature. Examples of such charts for: Stepped shafts in tension, bending, and torsion A plate with opposite Ushaped notches in tension and bending Elastic stress concentration factors depend only on geometry (independent of material) and mode of loading, and that they only apply when the notch is under linear elastic deformation condition. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 14
15 Stepped shaft in tension, bending, and torsion Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 15
16 plate with opposite Ushaped notches in tension and bending Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 16
17 STRESS AND STRAIN CONCENTRATIONS AND GRADIENTS For qualitative estimates we can use an analogy between stresses or strains and liquid flow. Restrictions or enlargements in a pipe produce local increases in flow velocity somewhat similar to the local increases in stresses produced by changes in cross section. The designer will try to "streamline" the contours of parts as indicated in Fig Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 17
18 STRESS AND STRAIN CONCENTRATIONS AND GRADIENTS Consider for instance an elliptic hole in a wide sheet. Placed lengthwise with the forces or flow it produces less stress concentration and less flow interference than when it is placed crosswise. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 18
19 STRESS AND STRAIN CONCENTRATIONS AND GRADIENTS K t produced by an elliptic hole with principal axes 2a and 2b is: b K t a where b is the axis transverse to the tension force and r is the radius of curvature at the endpoint of b. With an ellipse 30 mm long and 10 mm wide the stress concentration is: K t = 7 if placed crosswise K t = 1.67 if placed lengthwise Other examples of mitigating stress concentrations are given in Fig b r Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 19 2a r 2b
20 Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 20
21 Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 21
22 Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 22
23 Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 23
24 Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 24
25 Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 25
26 Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 26
27 SN APPROACH FOR NOTCHED MEMBERS Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 27
28 SN APPROACH FOR NOTCHED MEMBERS Notch Sensitivity and the Fatigue Notch Factor, K f Effects of Stress Level on Notch Factor Mean Stress Effects and Haigh Diagrams Example of Life Estimation with SN Approach Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 28
29 SN APPROACH FOR NOTCHED MEMBERS (Notch Sensitivity and Fatigue Notch Factor, K f ) The effect of the notch in the stresslife approach is taken into account by modifying the unnotched SN curve through the use of the fatigue notch factor, K f. Notched fatigue strength not only depends on the stress concentration factor, but also on other factors such as the notch radius, material strength, and mean and alternating stress levels. The ratio of smooth to net notched fatigue strengths, based on the ratio of alternating stresses is called K f. K f = (Smooth fatigue strength) / (Notched fatigue strength) Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 29
30 SN APPROACH FOR NOTCHED MEMBERS (Notch Sensitivity and Fatigue Notch Factor, K f ) The fatigue notch factor, K f, is not necessarily equal to the elastic stress concentration factor. As a base for estimating the effect of other parameters we estimate the fatigue notch factor K f for zero mean stress and long life ( cycles). Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 30
31 SN APPROACH FOR NOTCHED MEMBERS (Notch Sensitivity and Fatigue Notch Factor, K f ) The difference between K f and K t is related to: Stress gradient: The notch stress controlling the fatigue life is not the maximum stress on the surface of the notch root, but an average stress acting over a finite volume of the material at the notch root. This average stress is lower than the maximum surface stress, calculated from K t When small cracks nucleate at the notch root, they grow into regions of lower stress due to the stress gradient. Localized plastic deformation at the notch root: The localized plastic deformation and notch blunting effect due to yielding at the notch root reduces the notch root stress, particularly at short lives. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 31
32 Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 32
33 SN APPROACH FOR NOTCHED MEMBERS (Notch Sensitivity and Fatigue Notch Factor, K f ) Values of K f for R = 1 generally range between 1 and K t, depending on the notch sensitivity of the material, q, which is defined by: q K K f t A value of q = 0 (or K f = 1) indicates no notch sensitivity, whereas a value of q = 1 (or K f = K t ) indicates full notch sensitivity. 1 1 The fatigue notch factor can then be described in terms of the material notch sensitivity as K f = 1 + q (K t  1) Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 33
34 SN APPROACH FOR NOTCHED MEMBERS (Notch Sensitivity and Fatigue Notch Factor, K f ) Neuber has developed the following approximate formula for the notch factor for R = 1 loading: q 1 1 r or K f 1 1 K t 1 r where r is the radius at the notch root. The characteristic length depends on the material. Values of for steel alloys are shown in Fig. 7.7, and a few values of for aluminum alloys are given as follows: S u, MPa (ksi) 150 (22) 300 (43) 600 (87), mm (in.) 2 (0.08) 0.6 (0.025) 0.4 (0.015) Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 34
35 Values of for steel alloys Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 35
36 SN APPROACH FOR NOTCHED MEMBERS (Notch Sensitivity and Fatigue Notch Factor, K f ) Peterson has observed that good approximations for R = 1 loading can also be obtained by using the somewhat similar formula: q 1 1 a r where a is another material characteristic length. or An empirical relationship between S u and a for steels is given as: K f 1 K 1 t a r 1 or a S u 1.8 with S u in Mpa and a in mm a S u 1.8 with S u in ksi and a in inches For aluminum alloys, a is estimated as mm (0.025 in.). Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 36
37 SN APPROACH FOR NOTCHED MEMBERS (Notch Sensitivity and Fatigue Notch Factor, K f ) The formulas to estimate K f, such as those by Neuber and Peterson, are empirical in nature. These formulas express the fact that for large notches with large radii we must expect K f to be almost equal to K t, but for small sharp notches we may find K f << K t (little notch effect) for metals with ductile behavior, although K f remains large for high strength metals. In general, hard metals are usually more notch sensitive than softer metals. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 37
38 SN APPROACH FOR NOTCHED MEMBERS (Effects of Stress Level on Notch Factor) In the absence of data the behavior of notched parts must be estimated. For fatigue life of 10 6 to 10 8 cycles with R = 1 we can estimate the notched fatigue strength as S f /K f. At 1 cycle (approximately a tensile test) the monotonic tensile strength of the notched part for a metal behaving in a ductile manner can be estimated to be equal to the strength of the smooth part in monotonic testing. A straight line between these points, Basquin's equation, in a log Slog N plot is a reasonable approximation unless other data are available. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 38
39 SN APPROACH FOR NOTCHED MEMBERS (Effects of Stress Level on Notch Factor) An SN curve for fully reversed stresses for notched parts can thus be estimated from the following data: The ultimate tensile strength, S u, or true fracture strength, f, of the material. The long life fully reversed fatigue strength, S f, for smooth specimens of comparable size. The material characteristic length a or. The elastic stress concentration factor, K t, and radius, r, of the notch. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 39
40 EXAMPLE For an 80 mm wide sheet of 1020 hotrolled steel with a 10 mm central hole, construct the SN curve. 80 mm 10 mm Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 40
41 EXAMPLE From Table A.1: S f = 241 MPa at approximately 10 6 cycles S u = 448 MPa. Define the smooth line from 448 MPa at 1 cycle to 241 MPa at 10 6 cycles. 80 mm From Fig. 7.1: K t = 2.7, and From Fig. 7.7, = 0.24 mm. Then: 10 mm K f 1 1 K t 1 r Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 41
42 EXAMPLE The SN line for the sheet with the hole then goes from 448 MPa at 1 cycle to 241/2.4 = 100 MPa at 10 6 cycles. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 42
43 SN APPROACH FOR NOTCHED MEMBERS (Effects of Stress Level on Notch Factor) It should be noted that for metals behaving in a brittle manner, the notch effect at short lives is usually more pronounced than that presented in Fig An alternative estimate of the SN curve for a notched member made of a ductile material assumes equal fatigue strengths of the notched and smooth members at 10 3 reversals (discussed later in the next section). Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 43
44 SN APPROACH FOR NOTCHED MEMBERS Mean Stress Effects and Haigh Diagram Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 44
45 SN APPROACH FOR NOTCHED MEMBERS (Mean Stress Effects and Haigh Diagram) Figure 7.9 shows the fatigue strengths of smooth and notched specimens of T6 AL alloy at 10 4 and at 10 7 cycles plotted versus the mean stress. Elastic stress concentration factor was 3.4. From Fig. 7.9, values of the fatigue notch factor, K f, are shown below. At 10 4 cycles At 10 7 cycles At zero mean stress K f = 51/22 = 2.3 K f = 22/10 = 2.2 At 172 MPa mean stress K f = 42/13 = 3.2 K f = 17/3 = 5.7 Obviously not only is the fatigue notch factor not equal to the elastic stress concentration factor, but it also changes with the mean stress and cycles to failure. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 45
46 SN APPROACH FOR NOTCHED MEMBERS (Mean Stress Effects and Haigh Diagram) Figure 7.10 shows lines for median fatigue life of 10 6 cycles for smooth parts and for notched parts with K f = 2.9 for this material in terms of alternating stress S a versus mean stress S m. Note the great variation in the ratio K f of notched parts as compared to the smooth parts. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 46
47 SN APPROACH FOR NOTCHED MEMBERS (Mean Stress Effects and Haigh Diagram) On the compression side K f decreases to less than 1 at greater compressive mean stress, which means that a part with a groove may be stronger than a smooth part! (due to compressive residual stresses discussed in Ch 8). The diagram in Fig is typical. Similar diagrams can easily be constructed for other materials and other values of K f. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 47
48 SN APPROACH FOR NOTCHED MEMBERS (Mean Stress Effects and Haigh Diagram) The important points to remember are: Mean stress has more effect in notched parts than in smooth specimens. Tensile mean stress can increase the fatigue notch factor K f above the stress concentration factor K t and can be fatal in fatigue loading. Compressive mean stress can significantly reduce and even eliminate the effects of stress concentrations and save parts. Mean stresses inherent in the unloaded part due to residual stresses are often much greater than mean stresses caused by external loads. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 48
49 SN APPROACH FOR NOTCHED MEMBERS (Mean Stress Effects and Haigh Diagram) The SN approach for the combined effects of the mean stress and the notch is based on the use of available or estimated Haigh diagrams (constant life diagrams), such as that shown in Fig From such diagrams one point of an SN curve is obtained. A second point for the SN curve is obtained from knowledge or estimate of the stress corresponding to a very short life, usually either 1 or 1000 cycles. These points are joined by a straight line on log Slog N coordinates. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 49
50 SN APPROACH FOR NOTCHED MEMBERS (Mean Stress Effects and Haigh Diagram) To estimate a Haigh diagram, the following data must be either available or estimated: The monotonic yield strength, S y. The cyclic yield strength, S y. The unnotched fully reversed fatigue limit, S f, or the fatigue strength at about 10 6 to10 8 cycles. The true fracture strength, f. The fully reversed long life fatigue notch factor, K f. The critical alternating tensile stress, S cat. The critical alternating tensile stress, S cat, is the stress below which cracks will not propagate. It is estimated as 70 MPa (10 ksi) for hard steel, 30 MPa (4 ksi) for mild steel, and 20 MPa (3 ksi) for high strength aluminum. However, if any margin for safety is used, S cat can be taken as zero in design. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 50
51 SN APPROACH FOR NOTCHED MEMBERS (Mean Stress Effects and Haigh Diagram) Construction of the Haigh diagram is shown in Fig Any combination of mean and alternating stresses outside the triangle from S y to S y to +S y corresponds to gross yielding. Any combination above the line AB will produce a median fatigue life less than 10 6 to 10 8 cycles for smooth parts. For a part with a notch, the estimated Haigh diagram is shown by lines FCDE. The presence of tensile mean stress reduces the amount of alternating stress that can be tolerated. Maximum alternating stress can be tolerated with a sufficient compressive mean stress (Point F). Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 51
52 SN APPROACH FOR NOTCHED MEMBERS (Mean Stress Effects and Haigh Diagram) A simple approach for estimating the long life fatigue strength with a mean stress which does not require construction of the Haigh diagram is use of the modified Goodman equation. For a notched member, the long life smooth fatigue strength is simply divided by the fatigue notch factor, K f : S S a S m / K S f f u 1 The estimates for both smooth and notched parts based on the modified Goodman equation along with the yield limits are shown in Fig Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 52
53 Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 53
54 SN APPROACH FOR NOTCHED MEMBERS (Mean Stress Effects and Haigh Diagram) With diagrams like those in Figs or 7.12 the longlife fatigue strength of parts with notches for any combination of mean and alternating stresses can be estimated. For an estimate of a short life at a high stress: Static fracture is one point that can be used, based on a monotonic fracture test. A conservative estimate for metals with ductile behavior equates the nominal fracture stress in the part to S u, or f. Another prediction can be obtained by assuming that smooth and notched parts of metals with ductile behavior have equal nominal fatigue strengths at 1000 reversals or 500 cycles. One can interpolate by assuming a straight line between these points on an SN diagram on logarithmic scales (Basquin's Eq.). Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 54
55 EXAMPLE OF SN APPROACH FOR A NOTCHED MEMBER WITH MEAN STRESS Construct SN lines for (a) completely reversed loading (b) loading with minimum nominal stress of 50 MPa Material is QT hotrolled ROC100 steel Table A.2: S u = 931 MPa, S y = 883 MPa, f = 1330 MPa, S y = 600 MPa, f = 1240 MPa, and b = K t = 3 The nominal stress S = P/A + Mc/I = 11.25P (MPa), where P is the load in kn. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 55
56 EXAMPLE OF SN APPROACH FOR A NOTCHED MEMBER WITHOUT MEAN STRESS Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 56
57 EXAMPLE OF SN APPROACH FOR A NOTCHED MEMBER WITH MEAN STRESS Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 57
58 STRAINLIFE APPROACH FOR NOTCHED MEMBERS Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 58
59 STRAINLIFE APPROACH Notch Stresses and Strains Notch Strain Analytical Methods Linear rule Neuber s rule Strain energy density or Glinka s rule Plane Stress versus Plane Strain Example Problem Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 59
60 STRAINLIFE APPROACH A common application of the strainlife approach is in fatigue analysis of notched members, because: the deformation of the material at the notch root is often inelastic. notch stresses and strains are explicitly considered in the strainlife approach, whereas the SN approach is only in terms of nominal stresses. An example where significant notch plastic deformation and mean stresses are present is in variable amplitude loading with overloads and during low cycle fatigue. Application of the strainlife approach involves two steps: determination of local (notch) stresses and strains. life prediction using the local stresses and strains, based on the strainlife equation and analysis discussed in Chapter 5. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 60
61 Notch Stresses and Strains Notch root and nominal stresses and strains represented by ( ) and (S, e) are defined and shown. If the metal at the notch root is strained beyond the yield strength it may strain harden and cyclic harden or soften as discussed in Chs 3 and 5. As long as stresses and strains at the notch root remain elastic we have: = K t S = K t e Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 61
62 Notch Stresses and Strains The loads on notched parts are often sufficiently high such that the local stress: is considerably above the yield strength is less than K t S stresses are no longer proportional to strains. We then define strain and stress concentration factors as: K e K S Variations of stress and strain concentration factors with notch stress is shown in Fig Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 62
63 Variations of stress and strain concentration factors with notch stress Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 63
64 Notch Stresses and Strains The relation between and is given by the monotonic stressstrain curve, often represented by the Ramberg Osgood equation: 1 / n e p E K Values for n and K can be taken from Table A.2. Given nominal elastic stress S or strain e, the local stress and the local strain at the notch root can be obtained by: experimental methods, finite element methods, analytical models Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 64
65 Notch Stresses and Strains Experimental methods were discussed in Section 7.1. Finite element method requires small element size in high stress gradient regions a realistic representation of the nonlinear material stressstrain behavior (such as RambergOsgood equation). Analytical models Require the value of elastic stress concentration factor, K t (for complex geometries linear FEA can be used to obtain K t ). Include the linear rule, Neuber's rule, and strain energy density or Glinka's rule. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 65
66 LINEAR RULE The linear rule is expressed as: K K t e or = K t e For nominal elastic behavior, e = S/E The notch strain,, can be computed directly and, if desired, the notch stress,, can then be obtained from the stressstrain curve (or RambergOsgood Equation). For cyclic loading, notch and nominal stresses and strains are replaced by their respective ranges. The linear rule agrees with measurements in plane strain situations, such as circumferential grooves in shafts in tension or bending. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 66
67 Neuber s Rule Neuber's rule is the most widely used notch stress/strain model. It is expressed as: K K = K t 2 or = K t 2 e S According to this relation, the geometrical mean of the stress and strain concentration factors under plastic deformation conditions remains constant and equal to the theoretical stress concentration factor, K t. See Fig This rule agrees with measurements in plane stress situations, such as thin sheets in tension. Application of this rule requires the solution of two simultaneous equations (the above equation which describes a hyperbola, and the stressstrain equation). Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 67
68 Application of Neuber s rule for monotonic loading using a graphical method, where point A is the solution Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 68
69 Neuber s Rule For nominal elastic behavior, e = S/E: = K t 2 e S and Neuber's rule results in: 2 K t S E Combining this equation with the stressstrain equation results in E 2 K 1 / n 2 K t E S This equation can be solved for notch stress, iteration or numerical techniques, by Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 69
70 Neuber s Rule For cyclic loading: The monotonic stressstrain curve is replaced by the hysteresis curve and the strains and stresses are replaced by the strain ranges and stress ranges. Based upon better agreement with experimental fatigue life results, the fatigue notch factor, K f, is used in place of the theoretical stress concentration factor, K t. Neuber's rule for computing then is: = K f 2 e S For nominal elastic behavior, e = S/E, and 2 K f S Analogous to monotonic loading: E E K 1 / n 2 K S f E Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 70
71 Neuber s Rule Illustration of Neuber's rule for cyclic loading. Use of the cyclic stressstrain curve assumes stable cyclic behavior. Note that for unloading, the point of reversal S 1 is used as the origin of the Neuber hyperbola and the hysteresis curve, not = 0. For the continued constant amplitude loading, the notch stress and strain will continue to follow the closed hysteresis loop shown. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 71
72 Neuber s Rule Knowing, and max, we can obtain a =, and m = max . Notch strain amplitude, a, and notch mean stress, m, are then used for life prediction analysis. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 72
73 Strain Energy Density or Glinka s Rule This rule is based on the assumption that strain energy density at the notch root is nearly the same for linear elastic notch behavior (W e ) and elasticplastic notch behavior (W p ), as long as the plastic deformation zone at the notch is surrounded by an elastic stress field. For nominal elastic stress, S, the nominal strain energy density, W S, is given by (with e = S/E and de = ds/e): W s e 0 S de S 0 S E ds S 2 2 E Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 73
74 Strain Energy Density or Glinka s Rule At the notch root with a stress concentration factor of K t, strain energy density assuming linear elastic behavior ( = K t S and = /E) is: W e e 0 d 0 e E d 2 e 2 E K t S 2 E 2 For elasticplastic behavior at the notch root, the stressstrain relationship can be expressed by RambergOsgood equation and the strain energy density is given by: W p d 2 E n K 1 / n Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 74
75 Strain Energy Density or Glinka s Rule Setting W p = W e results in: / n 2 K t S E n 1 K E For a given nominal stress S, notch stress calculated. can be The only difference with Neuber's rule is the factor [2/(n+1)]. Since n < 1, smaller notch stress (and therefore smaller notch strain) is predicted based on this equation than from Neuber's rule). Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 75
76 Strain Energy Density or Glinka s Rule For cyclic loading, the equation is written in terms of stress and strain ranges and material monotonic deformation properties (K and n) are replaced by cyclic deformation properties (K and n ): / n 2 K t S E n 1 2 K E This equation relates nominal stress range, S, to notch stress range,. Notch strain range,, is then found from the hysteresis loop equation and used in the strainlife equations to find the fatigue life, similar to the procedure for Neuber's rule. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 76
77 Plane Stress versus Plane Strain The notch strain analysis presented assumed a uniaxial state of stress at the notch root. This condition exists for a plane state of stress such as in a thin plate. For plane strain conditions such as in a thick plate, however, the state of stress is no longer uniaxial, because in the thick plate the surrounding elastic material restrains notch deformation in the thickness direction, z 0, resulting in a stress z. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 77
78 Plane Stress versus Plane Strain For the plane strain conditions, a smaller notch strain range and a larger notch stress range in the loading direction results, as compared with the plane stress condition. Plane stress and plane strain conditions represent two bounding conditions which occur at the notch root. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 78
79 EXAMPLE OF LIFE ESTIMATION OF A NOTCHED MEMBER WITH N APPROACH Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 79
80 Example of Life Estimation with N Approach Notched part shown with K t = 3 and made of RQC100 steel. We want to find: (a) notch stress and strain from a 53.4 kn (12 kip) monotonic load, (b) notch stress and strain after unloading from the monotonic load in part (a) to zero, (c) notch stress and strain amplitudes from constant amplitude alternating loads between 4.45 kn (1 kip) and 44.5 kn (10 kip), and (d) the expected fatigue life to the formation of cracks on the order of 1 mm from the loading in part (c). Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 80
81 Example of Life Estimation with N Approach The relevant properties quoted from Table A.2 are: E = 207 GPa S y = 883 MPa K = 1172 MPa n = 0.06 S y = 600 MPa K = 1434 MPa n f = 1240 MPa ' f = b = c = Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 81
82 Example of Life Estimation with N Approach PART (a): Find notch stress & strain from a 53.4 kn monotonic load From Example 7.2.4, S = P = (53.4) = 600 MPa The nominal monotonic behavior is elastic, since S max = 600 MPa is about 2/3 of the yield strength, S y = 883 MPa. However, the monotonic notch root behavior is inelastic since K t S max = 3 x 600 = 1800 MPa > S y = 883 MPa. To find the notch root stress and strain using Neuber's rule, we have to solve the following two simultaneous equations: K t E S 2 3 x E K 1 / n / 0.06 resulting in: (See Fig. 7.23) = 903 MPa and = Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 82
83 Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 83
84 Example of Life Estimation with N Approach If strain energy density rule is used: E 2 n 2 1 K 1 / n 2 K t E S 2 3 x600 or: resulting in = 872 MPa / Substituting this value into the stressstrain equation results in: 2 E K 1 / n / These values are smaller than those predicted by Neuber's rule, as expected. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 84
85 Example of Life Estimation with N Approach If we used the linear rule, notch root strain and stress would be calculated as K t e K t E S 3 x / 0.06 or = 849 MPa Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 85
86 Example of Life Estimation with N Approach PART (b): Find notch stress and strain after unloading from the monotonic load in part (a) to zero For unloading, we can assume Masing behavior with a factor of two expansion of the monotonic stressstrain curve. Unloading is from S 1 = S max = 600 MPa to S 2 = 0, or S = 600 MPa. From Neuber's rule we obtain: K f S E 2 1 / n 3 x / 0.06 resulting in: = 1566 MPa, and = E 2 2 K Residual stress, min, and strain, min, after unloading are calculated as (and shown in Fig. 7.23) : min = max  = = 663 MPa, and  = = min = max Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 86
87 Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 87
88 Example of Life Estimation with N Approach Using the strain energy density rule: / n 2 K t S E n 1 2 K E Or x / x resulting in = 1524 MPa, and E 2 2 K 1 / n Therefore, min = max = = 652 MPa, and  = = min = max / Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 88
89 Example of Life Estimation with N Approach The linear rule does not result in a notch strain after unloading. Notch stress after unloading is calculated as: 1 / or = 1515 MPa Therefore: min = max = = 666 MPa. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 89
90 Example of Life Estimation with N Approach Part (c): Find notch stress and strain amplitudes from constant amplitude alternating loads between 4.45 kn and 44.5 kn. S max = P max = (44.5) = 500 MPa S min = P min = (4.45) = 50 MPa S a = (S max  S min )/2 = (50050)/2 = 225 MPa The nominal behavior for cyclic loading is also elastic since S max, S min, and S a are smaller than S y = 600 MPa. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 90
91 Example of Life Estimation with N Approach We first need to calculate notch root stress and strain at the maximum load. Using Neuber's rule we use the fatigue notch factor, K f = 2.82, which was calculated in Example 7.2.4: max max K f S E max x / n 1 / 0.14 max max E max K max max 1434 This results in max = 745 MPa, and max = Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 91
92 Example of Life Estimation with N Approach Unloading takes place from 500 MPa to 50 MPa, or S = 450 MPa. Therefore, from Neuber's rule we obtain: K f E S x / n 1 / 0.14 E 2 2 K resulting in = 1082 MPa, and = Therefore, min = max  = = 337 MPa, m = ( max + min )/2 = ( )/2 = 204 MPa and a = /2 = /2 = , a = /2 = 1082/2 = 541 MPa. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 92
93 Example of Life Estimation with N Approach Using the strain energy density rule, at maximum load: 2 max 2 max max 1 / n 2 K t S max E n 1 K E Or 2 max max 1 max / x which gives max = 712 MPa. Substituting this value into the cyclic stressstrain equation results in: max 1 / n max max E K / Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 93
94 Example of Life Estimation with N Approach For unloading: E 2 4 n 1 2 K 1 / n 2 K t E S or x / x resulting in = 1070 MPa, and E 2 2 K 1 / n / Therefore, min = max  = = 358 MPa, m = ( max + min )/2 = ( )/2 = 177 MPa and a = /2 = /2 = , a = /2 = 1070/2 = 535 MPa. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 94
95 Example of Life Estimation with N Approach If we use the linear rule: max K t S E max 3 x / max max 1434 or max = 663 MPa Then K t e K t E S 2 3 x / Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 95 or = 1045 MPa Therefore, min = max  = = 382 MPa, m = ( max + min )/2 = ( )/2 = 141 MPa and a = /2 = /2 = , a = /2 = 1045/2 = 523 MPa.
96 Example of Life Estimation with N Approach PART (d): Find the expected fatigue life to the formation of cracks on the order of 1 mm from the loading in part (c) We can use the SmithWatsonTopper mean stress parameter, or Morrow s mean stress parameters from Chapter 5. Here we choose the SmithWatsonTopper parameter: a 2 N 2 b 2 f b c N N max f f f f f E N f 0.76 Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 96
97 Results Are Summarized as Follows Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 97
98 It can be seen from this table that the most conservative fatigue life is obtained from Neuber's rule and the least conservative life from the linear rule, result from strain energy density rule falling in between. If K t rather than K f had been used in the application of Neuber s rule for cyclic loading, the notch stress amplitude would be 561 MPa rather than 541 MPa, the notch strain amplitude would be rather than , and the expected fatigue life would be 3950 cycles rather than 5750 cycles. Therefore, more conservative predictions are obtaind by using K t, as expected. The notch stress amplitudes obtained from notch stress/strain analysis models presented could also be used in conjunction with the SN approach. In this case, the SN line or equation for the smooth behavior should be used, since the effect of the notch is already incorporated in the stress amplitude. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 98
99 Since the minimum stress in Part (c) is 50 MPa, the fatigue lives predicted from the strainlife approach in this example can be directly compared to those from the SN approach in Section From Fig. 7.16, for a nominal stress amplitude of S a = 225 MPa, the predicted life using Basquin s equation for the notched part is about cycles based on the Haigh diagram approach for long life, and about cycles based on the modified Goodman equation. The remaining life (crack growth life from formation of a crack to fracture) of the notched part in this example problem can be estimated based on linear elastic fracture mechanics discussed in Chapter 6. This is done in the next section. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 99
100 CRACK GROWTH AT NOTCHES Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 100
101 CRACK GROWTH AT NOTCHES Deformation of the material at the notch root under cyclic loading is often inelastic. Thus, cracks often start from a notch under conditions of local plasticity. As the cracks continue to grow, they grow into the elastic stressstrain field of the notch, and with subsequent growth extend into the net section elastic stressstrain field of the specimen or component. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 101
102 CRACK GROWTH AT NOTCHES After the crack exceeds a certain length, usually 10 to 20 percent of the notch radius, the notch geometry has little influence on the elastic stressstrain field of the advancing crack. Crack growth through a notch stressstrain field may represent a major or minor portion of the total fatigue life. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 102
103 CRACK GROWTH AT NOTCHES Because the stressstrain field of a notch varies, FCG behavior also may vary as the crack grows through the different fields, as shown. For cracks growing in the plastic stressstrain field of a notch, FCG rates are initially high, but decrease as the crack grows further away from the notch root. After the crack grows out of the notch plastic zone, its length may no longer be small, and the crack growth behavior merges with the long crack growth curve. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 103
104 CRACK GROWTH AT NOTCHES Crack growth behavior for small cracks growing in the elastic stressstrain field of a notch is often similar to that for physically small cracks. Crack growth behavior in the plastic and elastic stressstrain field of the notch in general is a combination of the previous two conditions, assuming the crack is small, as the crack grows from the plastic to the elastic stressstrain field. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 104
105 CRACK GROWTH AT NOTCHES For a crack that nucleates from a shallow or blunt notch, the fatigue behavior is often dominated by crack nucleation. Conversely, a crack may nucleate from a sharp notch rather quickly due to the elevated stresses at the notch root but it may stop growing once the crack grows through the notchinfluenced region. For this condition, crack growth may dominate the fatigue behavior or total fatigue life. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 105
106 CRACK GROWTH AT NOTCHES To quantify the influence of the stressstrain field of a notch on crack growth, consider a very wide plate with a circular hole containing a pair of small throughthickness cracks as shown. When the length of the fatigue crack, l, is small compared to the radius of the circle, c, the stress intensity factor, K small, can be approximated by K 1.12 ( K S ) small t where S is the net section stress. l Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 106
107 CRACK GROWTH AT NOTCHES Once the crack has grown a sufficient distance from the hole, the stress intensity solution takes on the form: K long S a where a = c + l and S is based on the gross area. Thus, for long cracks, the width or diameter of the hole acts as part of the crack. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 107
108 CRACK GROWTH AT NOTCHES Figure 7.26b shows variation of K as a function of the crack length, l, normalized by the radius of the hole, c. An intersection point can be approximated which identifies a transitional crack length where K small can be used for crack lengths less than l and K long can be used for crack lengths greater than l : l 1.12 c K t 2 1 Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 108
109 CRACK GROWTH AT NOTCHES The stress intensity factor solutions presented are valid for situations where notch tip plasticity effects are negligible. When this is the case, l is usually a small fraction of the root radius,, of the notch or stress concentration, where usually 0.1 l 0.2. Even for conditions where small scale yielding prevails, FCG rates for cracks emanating from notches tend to be higher than their long crack counterparts, as previously shown. A contributing factor to this behavior is the absence or reduction in tensile residual plastic deformation (resulting from crack tip plasticity) in the wake of the crack because the crack is small. Less residual plastic deformation in the crack wake means less crack closure, a greater K eff, and thus higher FCG rates. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 109
110 CRACK GROWTH AT NOTCHES For small cracks contained within the local elastic stressstrain field of a notch, extrapolation of the Paris equation into region I may provide a reasonable approach to life prediction, the same as that presented in Section 6.8 for small cracks. For small cracks contained within the plastic stressstrain field of a notch, elasticplastic fracture mechanics (EPFM) may provide at least a partial solution to the differences observed between the behavior of small cracks emanating from notches and long cracks. However, the decreased driving force with increasing crack length typically observed for these types of cracks is difficult to account for using LEFM or EPFM without use of some type of crack closure model. Many attempts have been made to account for the anomalous fatigue crack growth from notches. While these models have proven useful, they have not provided a complete correlation between notch fatigue crack growth data and LEFM long crack growth data. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 110
111 THE TWO STAGE APPROACH Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 111
112 THE TWO STAGE APPROACH The life of a structure is often considered in two stages: Stage 1: Life to the formation of a crack that is on the order of 1 mm, crack nucleation. Stage 2: Life from this existing crack to failure, crack growth. In some situations, stage 2 may be negligible in comparison to stage 1 (i.e. rotating bending of a small notched shaft) on the other hand, cracks may be present. Stage 1 then becomes negligible in comparison to stage 2. Predictions of stage 1 are most commonly done using the N method. Predictions of stage 2 are done using LEFM. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 112
113 EXAMPLE OF THE TWO STAGE APPROACH In Section 7.3.5d, fatigue life calculations were made for stage 1 using the strainlife approach. We can predict the fatigue life associated with stage 2 (fatigue crack growth). The total fatigue life includes both fatigue crack nucleation life with a crack on the order of 1 mm (stage 1) and fatigue crack growth life (stage 2). Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 113
114 EXAMPLE OF THE TWO STAGE APPROACH To use LEFM for Stage 2 Fatigue Life Calculations, the stress intensity factor solution for the specimen geometry is required, which is given by [33]: K (0.247 w ) P a w a w a w 3 where P is in kn and K is in MPa m. This expression is applicable for a specimen thickness t equal to 9.5 mm and a/w between about 0.32 and 0.75, which corresponds to crack lengths a as measured from the load line of 30 to 70 mm. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 114
CH 6: Fatigue Failure Resulting from Variable Loading
CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).
More informationSTRAINLIFE (e N) APPROACH
CYCLIC DEFORMATION & STRAINLIFE (e N) APPROACH MONOTONIC TENSION TEST AND STRESSSTRAIN BEHAVIOR STRAINCONTROLLED TEST METHODS CYCLIC DEFORMATION AND STRESSSTRAIN BEHAVIOR STRAINBASED APPROACH TO
More informationFigure 1: Typical SN Curves
StressLife Diagram (SN Diagram) The basis of the StressLife method is the Wohler SN diagram, shown schematically for two materials in Figure 1. The SN diagram plots nominal stress amplitude S versus
More informationFATIGUE FROM VARIABLE AMPLITUDE LOADING. Ali Fatemi  University of Toledo All Rights Reserved Chapter 9 Variable Amplitude Loading 1
FATIGUE FROM VARIABLE AMPLITUDE LOADING Ali Fatemi  University of Toledo All Rights Reserved Chapter 9 Variable Amplitude Loading 1 FATIGUE FROM VARIABLE AMPLITUDE LOADING SPECTRUM LOADS AND CUMULATIVE
More informationStructural Integrity Analysis
Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces
More informationFatigue. 3. Final fracture (rough zone) 1. Fatigue origin. 2. Beach marks (velvety zone)
Fatigue Term fatigue introduced by Poncelet (France) 1839 progressive fracture is more descriptive 1. Minute crack at critical area of high local stress (geometric stress raiser, flaws, preexisting cracks)
More informationFATIGUE TESTS AND STRESSLIFE (SN) APPROACH
FATIGUE TESTS AND STRESSLIFE (SN) APPROACH FATIGUE TESTING LOADING TEST MACHINES SPECIMENS STANDARDS STRESSLIFE APPEROACH SN CURVES MEAN STRESS EFFECTS ON SN BEHAVIOR FACTORS INFLUENCING SN BEHAVIOR
More informationFatigue Testing. Objectives
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
More informationFatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY)
Fatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY) Ali Fatemi, Jonathan Williams and Farzin Montazersadgh Professor and Graduate
More information9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE
9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE A machine part or structure will, if improperly designed and subjected to a repeated reversal or removal of an applied load, fail at a stress much lower than
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationCompletely reversed, strain controlled fatigue tests of a steel alloy with E=210000 MPa resulted in the following data:
Kul49.4350 Fatigue o Structure Example solutions 5 Problem 51. Completely reversed, strain controlled atigue tests o a steel alloy with E=10000 resulted in the ollowing data: a a, (o the stable curve)
More informationRESIDUAL STRESSES AND THEIR EFFECTS ON FATIGUE RESISTANCE
RESIDUAL STRESSES AND THEIR EFFECTS ON FATIGUE RESISTANCE Ali FatemiUniversity of Toledo All Rights Reserved Chapter 8 Residual Stresses & Their Effects 1 RESIDUAL STRESSES AND THEIR EFFECTS ON FATIGUE
More informationME111 Lecture 16 1. ME111 Instructor: Peter Pinsky Class #16 November 1, 2000
Toda s Topics ME111 Instructor: Peter Pinsk Class #16 November 1, 2000 Introduction to linear elastic fracture mechanics (LEFM). Problem 3 A centercracked plate of AII 1144 steel ( C = 115MPa m ) has
More informationTensile fracture analysis of blunt notched PMMA specimens by means of the Strain Energy Density
Engineering Solid Mechanics 3 (2015) 3542 Contents lists available at GrowingScience Engineering Solid Mechanics homepage: www.growingscience.com/esm Tensile fracture analysis of blunt notched PMMA specimens
More informationMultiaxial Fatigue. Professor Darrell Socie. 20082014 Darrell Socie, All Rights Reserved
Multiaxial Fatigue Professor Darrell Socie 20082014 Darrell Socie, All Rights Reserved Outline Stresses around holes Crack Nucleation Crack Growth MultiaxialFatigue 20082014 Darrell Socie, All Rights
More informationDESIGN TO PREVENT FATIGUE
W H I T E P A P E R DESIGN TO PREVENT FATIGUE Overview In 1954, two crashes involving the world s first commercial airliner, the de Havilland Comet, brought the words metal fatigue to newspaper headlines
More informationEXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR PRODUCTION ON THE PIERCED FLAT SHEET METAL USING LASER FORMING PROCESS
JOURNAL OF CURRENT RESEARCH IN SCIENCE (ISSN 23225009) CODEN (USA): JCRSDJ 2014, Vol. 2, No. 2, pp:277284 Available at www.jcrs010.com ORIGINAL ARTICLE EXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR
More informationdifferent levels, also called repeated, alternating, or fluctuating stresses.
Fatigue and Dynamic Loading 1 Fti Fatigue fil failure: 2 Static ti conditions : loads are applied gradually, to give sufficient i time for the strain to fully develop. Variable conditions : stresses vary
More informationB. INTRODUCTION TO ASSESSMENT PROCEDURES FOR CRACKED COMPONENTS
B. INTRODUCTION TO ASSESSMENT PROCEDURES FOR CRACKED COMPONENTS 40 INTRODUCTION HOW ARE INTEGRITY, SECURITY OR CRITICAL CONDITIONS ANALYSED IN A CRACKED STRUCTURE? FRACTURE MECHANICS Critical conditions
More informationFAILURE MODES and MATERIALS PROPERTIES. Component failures. Ductile and Brittle Fracture COMPONENT FAILURES. COMPONENT FAILURE MODES examples:
FAILURE MODES and MATERIALS PROPERTIES MECH2300  Materials Lecture 10 R. W. Truss Materials Engineering R.Truss@uq.edu.au COMPONENT FAILURES Structures lectures es on component es cause response in component
More informationObjective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels.
IMPACT TESTING Objective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels. Equipment Coolants Standard Charpy VNotched Test specimens Impact tester
More informationNumerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope
Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,
More informationSolid Mechanics. Stress. What you ll learn: Motivation
Solid Mechanics Stress What you ll learn: What is stress? Why stress is important? What are normal and shear stresses? What is strain? Hooke s law (relationship between stress and strain) Stress strain
More informationStress Strain Relationships
Stress Strain Relationships Tensile Testing One basic ingredient in the study of the mechanics of deformable bodies is the resistive properties of materials. These properties relate the stresses to the
More informationAdam Zaborski handouts for Afghans
Tensile test Adam Zaborski handouts for Afghans Outline Tensile test purpose Universal testing machines and test specimens Stressstrain diagram Mild steel : proportional stage, elastic limit, yielding
More informationME 215 Engineering Materials I
ME 215 Engineering Materials I Chapter 3 Properties in Tension and Compression (Part III) Mechanical Engineering University of Gaziantep Dr. A. Tolga Bozdana www.gantep.edu.tr/~bozdana True Stress and
More informationMETU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B306) INTRODUCTION TENSION TEST Mechanical testing
More informationFatigue crack propagation
1 (20) Repetition Ð Crack initiation and growth Small cracks Shear driven Interact with microstructure Mostly analyzed by continuum mechanics approaches Large cracks Tension driven Fairly insensitive to
More informationPOWER SCREWS (ACME THREAD) DESIGN
POWER SCREWS (ACME THREAD) DESIGN There are at least three types of power screw threads: the square thread, the Acme thread, and the buttress thread. Of these, the square and buttress threads are the most
More informationME311 Machine Design
ME Machine Design Lecture 5: FullyReversing Fatigue and the SN Diagram W Dornfeld Oct26 Fairfield University School of Engineering Discovering Fatigue With the Industrial Revolution came the steam engine
More informationFlaw Size Acceptance Limits for a Stainless Steel Pressure Vessel
Flaw Size Acceptance Limits for a Stainless Steel Pressure Vessel Consuelo GuzmanLeong Lucius Pitkin, Inc. Richland, Washington, U.S.A. Frederic A. Simonen, Ph.D. Lucius Pitkin, Inc. Richland, Washington,
More informationGriffith theory of brittle fracture:
Griffith theory of brittle fracture: Observed fracture strength is always lower than theoretical cohesive strength. Griffith explained that the discrepancy is due to the inherent defects in brittle materials
More informationPlastic Behaviour  Tensile Strength
Plastic Behaviour  Tensile Strength Transition of mechanical behaviour from elastic to plastic depends upon the material type and its condition as tested (hotrolled, coldrolled, heat treated, etc.).
More informationFATIGUE CONSIDERATION IN DESIGN
FATIGUE CONSIDERATION IN DESIGN OBJECTIVES AND SCOPE In this module we will be discussing on design aspects related to fatigue failure, an important mode of failure in engineering components. Fatigue failure
More informationTensile Testing. Objectives
Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able
More informationIMPELLER FATIGUE ASSESSMENT USING AN SN APPROACH
ENGINEERING PAPER 524408 IMPELLER FATIGUE ASSESSMENT USING AN SN APPROACH Samuel Orr Engineering Analysis Manager Howden Technology AMCA International Engineering Conference Las Vegas, NV, USA 2 4 March
More informationFatigue :Failure under fluctuating / cyclic stress
Fatigue :Failure under fluctuating / cyclic stress Under fluctuating / cyclic stresses, failure can occur at loads considerably lower than tensile or yield strengths of material under a static load: Fatigue
More informationDistinguishing strength from toughness. Understanding fracture toughness.
Lecture notes version 20 Oct 2010 Chapter 8 Fracture and fracture toughness A fractured Liberty Ship 8.1 Introduction and synopsis Distinguishing strength from toughness. Understanding fracture toughness.
More informationLABORATORY EXPERIMENTS TESTING OF MATERIALS
LABORATORY EXPERIMENTS TESTING OF MATERIALS 1. TENSION TEST: INTRODUCTION & THEORY The tension test is the most commonly used method to evaluate the mechanical properties of metals. Its main objective
More informationσ y ( ε f, σ f ) ( ε f
Typical stressstrain curves for mild steel and aluminum alloy from tensile tests L L( 1 + ε) A =  A u u 0 1 E l mild steel fracture u ( ε f, f ) ( ε f, f ) ε 0 ε 0.2 = 0.002 aluminum alloy fracture
More informationUniaxial Tension and Compression Testing of Materials. Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng
Uniaxial Tension and Compression Testing of Materials Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng 3.032 Lab Report September 25, 2013 I. Introduction Understanding material mechanics
More informationMUKAVEMET KIRILMA HİPOTEZLERİ
1 MUKAVEMET KIRILMA HİPOTEZLERİ 17. Theories of failure or yield criteria (1) Maximum shearing stress theory (2) Octahedral shearing stress theory (3) Maximum normal stress theory for brittle materials.
More informationTorsion Tests. Subjects of interest
Chapter 10 Torsion Tests Subjects of interest Introduction/Objectives Mechanical properties in torsion Torsional stresses for large plastic strains Type of torsion failures Torsion test vs.tension test
More informationCalculating and Displaying Fatigue Results
Calculating and Displaying Fatigue Results The ANSYS Fatigue Module has a wide range of features for performing calculations and presenting analysis results. By Raymond Browell Product Manager New Technologies
More informationQuestion 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationFatigue Failure Due to Variable Loading
Fatigue Failure Due to Variable Loading Daniel Hendrickson Department of Computer Science, Physics, and Engineering University of Michigan Flint Advisor: Olanrewaju Aluko 1. Abstract Fatigue failure in
More informationAN EXPLANATION OF JOINT DIAGRAMS
AN EXPLANATION OF JOINT DIAGRAMS When bolted joints are subjected to external tensile loads, what forces and elastic deformation really exist? The majority of engineers in both the fastener manufacturing
More informationMechanical Properties  Stresses & Strains
Mechanical Properties  Stresses & Strains Types of Deformation : Elasic Plastic Anelastic Elastic deformation is defined as instantaneous recoverable deformation Hooke's law : For tensile loading, σ =
More informationσ = F / A o Chapter Outline Introduction Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? and Tension Compression Shear Torsion Elastic deformation Chapter Outline Introduction To understand and describe how materials
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationStress: The stress in an axially loaded tension member is given by Equation (4.1) P (4.1) A
Chapter 4. TENSION MEMBER DESIGN 4.1 INTRODUCTORY CONCEPTS Stress: The stress in an axially loaded tension member is given by Equation (4.1) P f = (4.1) A where, P is the magnitude of load, and A is the
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationB.TECH. (AEROSPACE ENGINEERING) PROGRAMME (BTAE) TermEnd Examination December, 2011 BAS010 : MACHINE DESIGN
No. of Printed Pages : 7 BAS01.0 B.TECH. (AEROSPACE ENGINEERING) PROGRAMME (BTAE) CV CA CV C:) O TermEnd Examination December, 2011 BAS010 : MACHINE DESIGN Time : 3 hours Maximum Marks : 70 Note : (1)
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationSheet metal operations  Bending and related processes
Sheet metal operations  Bending and related processes R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Table of Contents 1.QuizKey... Error! Bookmark not defined. 1.Bending
More informationFatigue Life Estimates Using Goodman Diagrams
Fatigue Life Estimates Using Goodman Diagrams by Robert Stone The purpose of this paper is to review the proper methods by which spring manufacturers should estimate the fatigue life of a helical compression
More informationMAE 20 Winter 2011 Assignment 5
MAE 20 Winter 2011 Assignment 5 6.7 For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the modulus of elasticity is 115 GPa (16.7 10 6 psi). (a) What is the
More informationCRITERIA FOR PRELOADED BOLTS
National Aeronautics and Space Administration Lyndon B. Johnson Space Center Houston, Texas 77058 REVISION A JULY 6, 1998 REPLACES BASELINE SPACE SHUTTLE CRITERIA FOR PRELOADED BOLTS CONTENTS 1.0 INTRODUCTION..............................................
More informationNonlinear Models of Reinforced and Posttensioned Concrete Beams
111 Nonlinear Models of Reinforced and Posttensioned Concrete Beams ABSTRACT P. Fanning Lecturer, Department of Civil Engineering, University College Dublin Earlsfort Terrace, Dublin 2, Ireland. Email:
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationYield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials. τ xy 2σ y. σ x 3. τ yz 2σ z 3. ) 2 + ( σ 3. σ 3
Yield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials Brittle materials are materials that display Hookean behavior (linear relationship between stress and strain) and which
More informationNote 5.1 Stress range histories and Rain Flow counting
June 2009/ John Wægter Note 5.1 Stress range histories and Rain Flow counting Introduction...2 Stress range histories...3 General...3 Characterization of irregular fatigue loading...4 Stress range histogram...5
More informationInvestigation of Stress Intensity Factor of Axial Compressor Blade of Helicopter
Investigation of Stress Intensity Factor of Axial Compressor Blade of Helicopter Neelesh V K Mr. Manjunath M V Mr. Devaraj Dept. of Mechanical Engineering Asst prof, Dept. of Mechanical Engineering Asst
More informationComparison of typical 3D printing materials [1]
Comparison of typical 3D printing materials [1] ABS Its strength, flexibility, machinability, and higher temperature resistance make it often a preferred plastic for engineers, and professional applications.
More informationTensile Testing Laboratory
Tensile Testing Laboratory By Stephan Favilla 0723668 ME 354 AC Date of Lab Report Submission: February 11 th 2010 Date of Lab Exercise: January 28 th 2010 1 Executive Summary Tensile tests are fundamental
More informationTheoretical and Practical Aspects of Thermo Mechanical Reliability in Printed Circuit Boards with Copper Plated Through Holes
Theoretical and Practical Aspects of Thermo Mechanical Reliability in Printed Circuit Boards with Copper Plated Through Holes Stefan Neumann, Nina Dambrowsky, Stephen Kenny Atotech Deutschland GmbH Berlin,
More informationPROPERTIES OF MATERIALS
1 PROPERTIES OF MATERIALS 1.1 PROPERTIES OF MATERIALS Different materials possess different properties in varying degree and therefore behave in different ways under given conditions. These properties
More informationCE591 Fall 2013 Lecture 26: Moment Connections
CE591 Fall 2013 Lecture 26: Moment Connections Explain basic design procedure for moment (FR) connections Explain considerations for connections in momentresisting frames for seismic demands Describe problems
More informationInteraction of Hydrogen and Deformation in 316L Stainless Steel
Proceedings of the SEM Annual Conference June 14, 2009 Albuquerque New Mexico USA 2009 Society for Experimental Mechanics Inc. Interaction of Hydrogen and Deformation in 316L Stainless Steel Bonnie R.
More informationLecture Slides. Chapter 8. Screws, Fasteners, and the Design of Nonpermanent Joints
Lecture Slides Chapter 8 Screws, Fasteners, and the Design of Nonpermanent Joints The McGrawHill Companies 2012 Chapter Outline Reasons for Nonpermanent Fasteners Field assembly Disassembly Maintenance
More informationUnit 48: Structural Behaviour and Detailing for Construction. Chapter 13. Reinforced Concrete Beams
Chapter 13 Reinforced Concrete Beams Concrete is a material strong in its resistance to compression, but very weak indeed in tension. good concrete will safely take a stress upwards of 7 N/mm 2 in compression,
More informationChapter 5 Bridge Deck Slabs. Bridge Engineering 1
Chapter 5 Bridge Deck Slabs Bridge Engineering 1 Basic types of bridge decks Insitu reinforced concrete deck (most common type) Precast concrete deck (minimize the use of local labor) Open steel grid
More information2. FRACTURE MECHANICS
2. FRACTURE MECHANICS Igor Kokcharov 2.1 DEFECTS Structural materials have inner defects such as cracks, which are extreme stress concentrators. There are technological defects shown in diagrams A and
More informationTorsion Testing. Objectives
Laboratory 4 Torsion Testing Objectives Students are required to understand the principles of torsion testing, practice their testing skills and interpreting the experimental results of the provided materials
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationELASTOPLASTIC ANALYSIS OF A HEAVY DUTY PRESS USING F.E.M AND NEUBER S APPROXIMATION METHODS
International Journal of Mechanical Engineering and Technology (IJMET) Volume 6, Issue 11, Nov 2015, pp. 5056, Article ID: IJMET_06_11_006 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=6&itype=11
More information1. Introduction. 2. Response of Pipelines
1. Introduction Blasting is common in the coal industry to remove rock overburden so that the exposed coal can be mechanically excavated. A portion of the blast energy released is converted to wave energy
More informationEffects of Sulfur Level and Anisotropy of Sulfide Inclusions on Tensile, Impact, and Fatigue Properties of SAE 4140 Steel
Paper 281434 Effects of Sulfur Level and Anisotropy of Sulfide Inclusions on Tensile, Impact, and Fatigue Properties of SAE 414 Steel Copyright 28 SAE International Nisha Cyril and Ali Fatemi The University
More informationBending, Forming and Flexing Printed Circuits
Bending, Forming and Flexing Printed Circuits John Coonrod Rogers Corporation Introduction: In the printed circuit board industry there are generally two main types of circuit boards; there are rigid printed
More informationEFFECTS OF SHOTPEENING ON HIGH CYCLE FRETTING FATIGUE BEHAVIOR OF Ti6Al4V
JOURNAL OF AERONAUTICS AND SPACE TECHNOLOGIES JANUARY 2003 VOLUME 1 NUMBER 1 (5164) EFFECTS OF SHOTPEENING ON HIGH CYCLE FRETTING FATIGUE BEHAVIOR OF Ti6Al4V Halil Ibrahim Air Services Schools and
More information3. AXIALLY LOADED MEMBERS
3 AXIALLY LOADED MEMBERS 31 Reading Assignment: Section 19 and Sections 81 and 82 of text Most axially loaded structural members carry some moment in addition to axial load  for this discussion, restrict
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME 2 ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS
ENGINEERING COMPONENTS EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS Structural members: struts and ties; direct stress and strain,
More informationMechanical Properties
Mechanical Properties Hardness Hardness can be defined as resistance to deformation or indentation or resistance to scratch. Hardness Indentation Scratch Rebound Indentation hardness is of particular interest
More informationBearing strength of stainless steel bolted plates in tension
NSCC29 Bearing strength of stainless steel bolted plates in tension G. KIYMAZ 1 1 Department of Civil Engineering, Istanbul Kultur University, Ataköy Campus, Bakırköy, Istanbul, Turkey ABSTRACT: A study
More informationDesign Analysis and Review of Stresses at a Point
Design Analysis and Review of Stresses at a Point Need for Design Analysis: To verify the design for safety of the structure and the users. To understand the results obtained in FEA, it is necessary to
More informationFrequency domain application of the HotSpot method for the fatigue assessment of the weld seams
Frequency domain application of the HotSpot method for the fatigue assessment of the weld seams Dr. Ing. Sauro Vannicola 1 sauro.vannicola@ch.abb.com Dr. Ing. Luigi De Mercato 2 luigi.demercato@ch.abb.com
More informationThe Influence of Magnetic Forces on the Stability Behavior of Large Electrical Machines
The Influence of Magnetic Forces on the Stability Behavior of Large Electrical Machines Dr. H. Sprysl, Dr. H. Vögele, ABB Kraftwerke AG, CH5242 Birr Dr. G. Ebi, SENSOPLAN GmbH, D79801 Hohentengen a.h.
More informationREINFORCED CONCRETE. Reinforced Concrete Design. A Fundamental Approach  Fifth Edition
CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach  Fifth Edition CONCRETE Fifth Edition A. J. Clark School of Engineering Department of Civil and Environmental Engineering
More informationPLASTIC DEFORMATION AND STRESSSTRAIN CURVES
PLASTIC DEFORMATION AND STRESSSTRAIN CURVES Introduction Background Unit: Plastic Deformation and StressStrain Curves In the last unit we studied the elastic response of materials to externally applied
More informationSPECIFICATIONS, LOADS, AND METHODS OF DESIGN
CHAPTER Structural Steel Design LRFD Method Third Edition SPECIFICATIONS, LOADS, AND METHODS OF DESIGN A. J. Clark School of Engineering Department of Civil and Environmental Engineering Part II Structural
More informationHow Management Decisions Make or Break Plant Uptime
How Management Decisions Make or Break Plant Uptime Abstract How Management Decisions Make of Break Plant Uptime: When you run machines above design rates that decision goes against all that we know about
More informationMAE 20 Winter 2011 Assignment 6
MAE 0 Winter 011 Assignment 6 8.3 If the specific surface energy for sodalime glass is 0.30 J/m, using data contained in Table 1.5, compute the critical stress required for the propagation of a surface
More informationCAD and Finite Element Analysis
CAD and Finite Element Analysis Most ME CAD applications require a FEA in one or more areas: Stress Analysis Thermal Analysis Structural Dynamics Computational Fluid Dynamics (CFD) Electromagnetics Analysis...
More informationFinite Element Modeling of Reinforced Concrete BeamColumn Bridge Connections
Finite Element Modeling of Reinforced Concrete BeamColumn Bridge Connections ACKNOWLEDGEMENTS............................................ xix CHAPTER 1: INTRODUCTION......................................................
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQF LEVEL 3 OUTCOME 1  LOADING SYSTEMS TUTORIAL 3 LOADED COMPONENTS
EDEXCEL NATIONAL CERTIICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQ LEVEL 3 OUTCOME 1  LOADING SYSTEMS TUTORIAL 3 LOADED COMPONENTS 1. Be able to determine the effects of loading in static engineering
More informationMATERIALS AND MECHANICS OF BENDING
HAPTER Reinforced oncrete Design Fifth Edition MATERIALS AND MEHANIS OF BENDING A. J. lark School of Engineering Department of ivil and Environmental Engineering Part I oncrete Design and Analysis b FALL
More informationMaster of Simulation Techniques. Lecture No.5. Blanking. Blanking. Fine
Master of Simulation Techniques Lecture No.5 Fine Blanking Prof. Dr.Ing. F. Klocke Structure of the lecture Blanking Sheared surface and force Wear Blanking processes and blanking tools Errors on sheared
More informationMATERIALS SELECTION FOR SPECIFIC USE
MATERIALS SELECTION FOR SPECIFIC USE1 Subtopics 1 Density What determines density and stiffness? Material properties chart Design problems LOADING 2 STRENGTH AND STIFFNESS Stress is applied to a material
More informationLecture 12: Fundamental Concepts in Structural Plasticity
Lecture 12: Fundamental Concepts in Structural Plasticity Plastic properties of the material were already introduced briefly earlier in the present notes. The critical slenderness ratio of column is controlled
More information